4 Lightweight Potential of Future Car Body Material Concepts
4.3 Potential of Aluminium 41
The following subsection describes a possible approach of assessing the weight reduction potential for a certain body component when aluminium is substituted for steel.
In order to compare the results, this approach is similar to the approach assessing the poten- tial of high-strength steel as described in the previous subchapter. Consequently, most of the boundary conditions are consistent:
• Typical, empirical ranges for weight reduction achievable by substitution of aluminium for steel have to be available.
• The yield strength of the aluminium alloy used for a certain component is determined proportional with the strength relevance of this component and the difference be- tween maximum yield strength available and minimum yield strength of aluminium. This is in order to apply high strength material according to the actual requirements. • The weight reduction potential decreases with increasing stiffness relevance, since it
is difficult to compensate for the decrease in stiffness caused by downgauging of highly stiffness relevant components. For reasons for comparability the relation be- tween weight reduction potential decrease and stiffness relevance in identical with the approach used for determination of the potential of high-strength steel. However, in
practice the higher wall thickness of aluminium components enables larger section in- crease for stiffness compensation without buckling issues.
• Differences in ultimate strain, formability and brittleness of aluminium grades are not considered.
• Package restrictions are not considered.
The maximum achievable weight reduction using aluminium in comparison to steel is diffe- rent for strength in crash dominated and stiffness dominated components. In addition, the actual weight reduction for strength in crash dominated components is depending on the yield strength of the substituted steel component. Empirical ranges of the achievable weight reduction when substituting aluminium for steel are provided by Hydro Aluminium [PED09]. Compared to a similar steel component using aluminium the weight of stiffness dominated components can be reduced by up to 50 % in a range starting from 0 %. The actual weight reduction depends on the shape of the part and the load case. The highest weight reduction can be achieved for thin-walled, plane structures. The lowest weight reduction can be achieved for beams. However in practice with respect to typical sections and loads of auto- motive beams the lower value for weight reduction is rather 30 %, not 0 %.
If the design of a component is dominated by the requirement for strength in crash, the achievable weight reduction when substituting aluminium for steel depends on several influ- encing factors. First of all, it has to be determined whether energy absorption, e.g. for crash boxes, or strength in terms of deformation resistance, e.g. for B-Pillars, is the main design criterion of the component. This is necessary since the achievable weight reduction is higher for energy absorbing components because of the strong influence of the sheet-thickness on both crush-force and buckling stability. In addition, the actual weight reduction is not only depending on the yield strength of the substituted steel component but also on the yield strength of the aluminium alloy used for substitution. This means for a steel component with the same yield strength different values of weight reduction can be achieved depending on the chosen yield strength of the aluminium alloy. The diagram at the top of Fig. 4-10 summa- rises the mentioned influencing factors in a simplified linear approach.
Current Yield Strength of Component Weight Reduction Regarding Strength Weight Reduction Regarding Stiffness Minimum Weight Reduction Range Regarding Stiffness 35 - 50 % Stiffness Relevance of Component
Weight Reduction Potential of Component
Strength Relevance of
New Yield Strength of Component 0 10 20 30 40 50 60 70 0 200 400 600 800 1000 1200 1400 W eight R educ tion [% ]
Strength of Steel Component [MPa]
Strength Dominated Components Maximum Strength Dominated Components Minimum Energy Absorbing Components Maximum Energy Absorbing Components Minimum
Fig. 4-10: Flow scheme of approach for weight reduction assessment (aluminium)
For strength dominated components a weight reduction of 66 % defined by the density ratio of aluminium and steel can be achieved until the yield strength of steel exceeds the maxi- mum available yield strength of aluminium. Then the achievable weight reduction decreases and is equal to zero for yield strength of steel that is three times the aluminium yield strength, since the stresses have to be reduced by upgauging. The regression lines for energy absorb- ing components are determined by numerical and experimental studies.
The approach for assessment of the weight reduction potential of aluminium as shown by the flow scheme in Fig. 4-10 is similar to the approach for high-strength steel shown in Fig. 4-9. As the flow scheme in Fig. 4-10 indicates, the possible weight reduction for a certain compo- nent is determined separately for equivalent strength and equivalent stiffness. The minimum of both is regarded as the possible weight reduction for the specific component, since this defines the critical dimensioning.
In order to determine the weight reduction possible for equivalent stiffness of the component the maximum and minimum achievable weight reduction is defined by the range from 30 % to 50 % as described above [PED09]. The actual weight reduction for a certain component with regard to stiffness can be calculated based on the stiffness relevance of the component and the above described correlation between weight reduction and stiffness relevance. A linear approach is used in this case.
In the approach proposed two steps are required for determination of the achievable weight reduction for equivalent strength. First, an appropriate material strength is calculated for the specific component. As mentioned above, this is done by increasing the material strength linearly with the strength relevance of the component. For strength dominated components the yield strength of the aluminium alloy used can vary in a range from 250 MPa to 400 MPa while the range for energy absorbing components is from 150 MPa to 250 MPa. However, if the yield strength of the substituted steel component is lower than the minimum aluminium yield strength, the yield strength of the steel component is selected for the aluminium com- ponent. In the subsequent step the possible weight reduction can be calculated using the yield strength of the aluminium component, the yield strength of the substituted steel compo- nent and the according regression line from the diagram shown at the top of Fig. 4-10.
For the SLC-reference vehicle the required input data for the approach described above is available. Therefore, the approach can exemplarily be applied for the structure of this vehi- cle. This enables a comparison of the assessed weight reduction potential of a high-strength steel intensive vehicle as described in the previous subchapter to the weight reduction poten- tial of a full aluminium vehicle. In addition, the results can serve as a basis to identify suitable components for aluminium application in a multi-material design approach.
Following the approach the achievable weight reduction when substituting aluminium for steel in a state-of-the-art car body including closures is assessed to be 40 %. The average yield strength of the aluminium car body is with 244 MPa lower than the average yield strength of the steel car body with 338 MPa. Like for the high-strength steel intensive car body it has to be mentioned, that for the components limited by the stiffness requirement the new yield strength could be decreased.
The weight reduction potential of 40 % can be regarded to be at the upper limit. In practice, additional aspects will have to be considered such as the joinability, the performance of the joints or nodes connecting the different components or the NVH performance. Therefore it may not be possible to fully exploit the indicated weight reduction potential of high strength
aluminium alloys. However, similar restrictions may also apply to the substitution of ultra- high-strength steel grades for conventional steel grades.
It has to be mentioned that in contrast to perpetually mentioned arguments the weight reduc- tion potential of aluminium is limited by strength requirements for few components, only. The reason is that even in state-of-the-art car bodies most of the steel components are still made from steel grades that show yield strength in ranges that aluminium can compete with. This situation can be regarded to change in the future only to a limited extent, since many compo- nents are not suitable for efficient high-strength material usage. For many components stiff- ness will maintain the decisive criterion.
It can be expected that in future body concepts mountable components will have the best chances to be made of light materials. If lightweight design becomes more important due to emission regulations the market penetration of aluminium closures in the middle class and the compact class is a realistic scenario.